Experimental Investigation of Lime Treated Palm Kernel Shell and Sugarcane Bagasse Ash as Partial Replacement of Coarse Aggregate and Cement Respectively in Concrete

This experimental research is focused on the effect of concrete made by incorporating lime treated Palm Kernel Shell (PKS) & Sugarcane Bagasse Ash (SCBA) as partial replacements of coarse aggregates and Ordinary Portland Cement (OPC) respectively. An experimental analysis for concrete grade 30 with a mix design ratio of 1:1.97:3.71 of cement:fine aggregates:coarse aggregates with a constant water to cement ratio of 0.5, was used. Physical tests such as workability on fresh concrete and water absorption on hardened concrete of each batch were carried out. Mechanical tests like compressive strength and split tensile strength were carried out on hardened concrete cubes (100 mm × 100 mm × 100 mm) and cylinders (100 mm × 200 mm) at 7 and 28 days. The experimental results obtained in this study indicate the possibility of using up 15% of lime treated PKS and 10% of SCBA for production of structural concrete.


Introduction
Concrete is a manmade composite material consisting of cement, aggregates and water, which is used in civil engineering construction and is preferred all over the world.It is the second most consumed substance on earth after water [1].
According to [2] its usage is around 10 billion tons per year, which is equivalent to 1 ton per every living person and 1.7 tons per person in the United States.About 50% -80% of its volume are aggregates that consist of natural crushed stones and sand.Due to the depletion of natural resources, worry is gaining place in the construction industry.In addition, since the bonding material in the concrete is cement, the high demand for this material has led to an increase in cost, making it the most expensive construction material.In view of the magnitude of these problems, combined with the problem of waste disposal, researchers decided to look for other ecological materials that could be used in the production of concrete.
The incorporation of agricultural waste material for concrete production can considerably reduce the cost incurred in buying coarse aggregate, which results in a potential reduction in the total cost of construction and will also reduce environment pollution [3].Industrial actions produce significant quantities of non-biodegradables solid waste.Most of this waste consists of industrial waste (such as, sandpaper, chemical solvents, industrial by products, paints, paper products, metal and radioactive waste), municipal waste (such as plastics), and agricultural waste (natural fibers and such as palm kernel shell).
Palm kernel is the edible seed of the oil palm fruit.The fruit yields two distinct oils: palm oil derived from the outer parts of the fruit, and palm kernel oil derived from the kernel (FAO, 2002).Considerable amount of waste in form of PKS is generated during oil extraction.A PKS is an interesting alternative for combating problems of overexploitation of conventional aggregates in concrete whose global production increases regularly.The efforts of researchers are to achieve how to use that waste materials in concrete.

Materials and Methods
Ordinary Portland cement Type I (CEM I 42.5N) conforming to the requirements of [4] was used as a binding agent.According to [5], the treatment of PKS with lime reduce the amount of it water absorption.Hence, the Palm Kernel Shell obtained from Uganda at Kalangala island was treated with lime to make the shell less permeable.The treatment was done by putting PKS in lime solution (40 g/l) for 2 hours follow by air drying to obtain saturated surface dried such that the water cement ratio was not affected.It met the requirement of [6].The coarse and fine aggregate were locally obtained with nominal size of 20 mm for coarse aggregate and maximum size of 5 mm for fine aggregate.Both aggregates met the requirement of [6].The Sugar Cane Bagasse Ash used was locally obtained from sugar manufacturing industry in Kakamega County (KENYA) and was prepared by sieving on 0.075 mm sieve.It met the requirement of [7].The mix ratio of 1:1.97:3.71for cement:fine aggregates:coarse aggregates with a constant water to cement ratio of 0.5 was used.The target grade of concrete was C30 and the specimens size used was cubes (100 mm ×

Material Characteristics
The characteristics of PKS, SCBA, OPC, coarse and fine aggregates are in terms of Aggregate Crushing Value (ACV), Aggregate Impact Value (AIV), compressive strength, density, particle size distribution, specific gravity, splitting tensile strength, water absorption, and workability.

Characterization of PKS, Coarse Aggregate and Fine Aggregate
The particle size distribution of coarse aggregate and PKS are presented in   As presented in Figure 3, the particles size of fine aggregates was between 0.15 to 4.75 mm.It can be seen that the particles of fine aggregates satisfied the re-Open Journal of Civil Engineering quirements of [6], which requires that the fine aggregate be less the 45% retained on any one sieve.As shown in Table 1, although the water absorption of treated PKS is lower than untreated PKS, both are higher than the water absorption of coarse aggregate.This high-water absorption of treated PKS could lead to poor concrete workability as the quantified water for a given concrete workability might be absorbed by the PKS.The specific gravity for coarse aggregate and PKS were 2.49 and 1.01 respectively.According to [8], aggregates with specific gravity less than 2.4 are classified as light-weight aggregate (LWA).Hence, PKS can be categorized as a light-weight aggregate (LWA) since his specific gravity is less than 2.4.The ACV for coarse aggregate and PKS satisfied [9] requirement since the maximum recommended was 30%.This induces that the PKS can be used for surface pavement.According to [10], the specified limit for AIV for aggregates which are adequate for concrete with good impact resistance is 25%.Therefore, PKS and coarse aggregate showed better impact resistance and are in adequation with [10].
For the fine aggregate, his specific gravity was 2.45 while the fineness modulus gested that the fineness modulus be kept between 2.3 and 3.1.This is due to the fact that a "very fine" fine aggregate will increase water demand on the mix, while a "very coarse" fine aggregate could compromise workability.Hence, the fineness modulus results obtained shows that the material was not very fine and not very coarse either, and therefore suitable for the production of concrete with high workability and finish-ability.

Characteristics of Sugarcane Bagasse Ash and Ordinary Portland Cement
The maximum particle size of SCBA used in this research was 0.075 mm (75 µm).
Its hydrometer analysis result is presented in

Chemical Analysis of Sugarcane Bagasse Ash and Ordinary Portland Cement
As shown in Table 2, the silica (SiO 2 ) content of SCBA is 297% higher than that of cement while the free lime content (CaO) of cement is higher than SCBA by 94.86%.Despite this, we noted that the SCBA satisfied the minimum requirement of [7] which required 70% for a good pozzolana.
Therefore, the presence of silica and alumina above the minimum requirement for a good pozzolana shows the ability of the SCBA to form cementitious compound when mixed with the free lime of the OPC in the presence of moisture.Calcium oxide is required for the formation of Tricalcium silicate and Dicalcium silicate which both reacts with water to form Calcium silicate hydrate which gives concrete its strength.

Workability of Lime Treated PKS and SCBA Concrete
Workability in terms of slump test is presented in Figures 5-7.From Figure 5, though the PKS was treated with lime to reduce the water absorption, there was still a reduction in slump with increase in PKS content.The workability reduced from 27 mm for the control mix to 20 mm for 20% addition of PKS.This might have been due to the finer particle sizes of PKS when compared to the coarse aggregate.From Figure 6, the presence of SCBA in the mix resulted in increased amount of fines as seen by the Particle Size Distribution curve of the SCBA concrete mix which increased the water demand for the mix.It confirms to the fact that pozzolanic reactions require more water as compared to normal concrete made with OPC.This finding is consistent with the research outcomes [11], which reported the reduction in slump with increase in percentage of SCBA.
As presented in Figure 7, it can be seen that the workability of lime treated PKS & SCBA concrete decreased at all mixes when compare to normal weight concrete.
The lowest workability recorded falls in the very low range (0 -25 mm).The decrease in workability of lime treated PKS & SCBA concrete can be seen to be   Consequently, when using both lime treated PKS & SCBA, superplasticizers should be used in order to improve the workability of the concrete.

Water Absorption of Lime Treated PKS and SCBA Concrete
The water absorption of lime treated PKS concrete increased slightly as the percentage replacement of lime treated PKS increase as shown in Figure 8.At 0% Open Journal of Civil Engineering the water absorption was 1.72%, which increased to 3.74% at 20% PKS addition.
This reduction in workability can be attributed to increase in the water absorption of the mix which must have resulted in the presence of voids in the hardened concrete.It is in order with the report of [12].Similar result was obtained from Figure 9 for SCBA concrete which shows a rise in the water absorption of concrete as the percentage of SCBA increases from 1.72% in the control to 2.80% at 20% SCBA content.This is due to the high absorptivity characteristic of SCBA as it particles was very fine.

Density of Lime Treated PKS and SCBA Concrete
The hardened bulk density of all lime treated PKS concrete and SCBA concrete prepared in this study are graphically presented in Figure 11 & Figure 12.The density of lime treated PKS concrete increased from 7 days to 28 days while decreased as the percentage of substitution increased.This can be attributed to the low specific gravity of PKS which lead to porous concrete and can reduce the compressive strength.Similar results were observed on density of SCBA concrete.
It could be as a result that SCBA having a less bulk density of 554.13 kg/m 3 as compared to that of OPC which was 1396.67 kg/m 3 .It is consistent with [11] who reported, the average density of concrete decreases with increase in percentage replacement of SCBA with cement.
From Figure 13, the hardened density of lime treated PKS & SCBA concrete increased from 7 to 28 days, although a decrease was noticed with increase in the percentage replacement.This reduction is expected as the constituent materials were observed to be lighter than their replacements.Also, it can be said that because of the reduction in slump, there must have been poor compaction which

Compressive Strength of Lime Treated PKS and SCBA Concrete
Compressive strength is the capacity of a material or structure to withstand loads tending to reduce size.The compressive strength of concrete is one of the most important and useful properties of concrete.In most structural applications, concrete is used primarily to resist compressive stresses.It is obtained by dividing the maximum load applied to the cube by the cross-sectional area [14].From the experimental investigation, the compressive strength of lime treated PKS concrete (Figure 14) shows that the concrete gains strength with an increase in the curing age as the 7 days strength was lower than 28 days but decreases with an increase in PKS replacement.aggregates thereby resulting into weak bonding as more cement paste might have been demanded.Again, since lime-pozzolana reactions required time, it could be that the 28 days curing period was not sufficient for the full development of the strength and thus resulting in the reduction of the compressive strength.
According to [16] a compressive strength within the range of 20 to 45 MPa is classified as good for normal weight concrete.Hence up to 15% of lime treated PKS and 10% of SCBA can be used as partial replacement of coarse aggregate and OPC respectively in production of structural concrete.

Splitting Tensile Strength of Lime Treated PKS and SCBA Concrete
The tensile strength of concrete is one of the basic and important properties which greatly affect the extent and size of cracking in structures.Concrete develops cracks when tensile forces exceed its tensile strength.A tensile strength is a measure of the ability of material to resist a force that tends to pull it apart.It is expressed as the minimum tensile stress (force per unit area) needed to split the material apart.As portrayed in Figure 17 & Figure 18 the evolution of splitting tensile strength, the experimental results show a trend that resembles the compressive strength results.The Splitting tensile strength of lime treated PKS concrete and SCBA concrete decreased as increased in percentage replacement while increased in curing age.This reduction can be attributed to poor compaction, increased surface area of the lime treated PKS, reduced bonding properties of SCBA in constituent materials in concrete as compared to the cement.This is in concordance with result reported by [15].
From Figure 19, the splitting tensile strength decreased from 3.00 MPa for the

Conclusions
From the experimental investigation of this research, the following conclusion can be made.

Fig- ure 1 &
Figure 2. The figure shows that 90% of Coarse aggregates and PKS sizes, were between 5 mm to 25 mm.Both of their curves were between upper and lower limit curve referenced in [6].From the graph, it was noticed that the particle size of PKS are closer to upper limit envelope, which mean that the PKS has various bigger size of particles and can lead to the production of concrete with many voids, or the use of a larger portion of fine aggregate to fill those voids between the aggregates.

Figure 1 .
Figure 1.Particle size distribution of coarse aggregate.

Figure 3 .
Figure 3. Particle size distribution of fine aggregate.

Figure 4 .
From the Figure, about 28% of it particles were between 0.002 mm (2 µm) to 0.02 mm (20 µm), and 72% between 0.02 mm (20 µm) to 0.065 mm (65 µm).Due to this finesse particle, the surface area and water demand of SCBA improved.In terms of specific gravity, the SCBA and OPC were 2.00 and 3.09 respectively.Due to the fact that the specific gravity was below 2.40, it can be said that the SCBA used in this research was lightweight material[8].The low specific gravity of SCBA can contribute in the reduction of concrete density.

Figure 8 .
Figure 8. Water absorption of lime treated PKS concrete.

Figure 10 .
Figure 10.Water absorption of lime treated PKS and SCBA concrete.

Figure 16 .
Figure 16.Compressive strength of lime treated PKS and SCBA concrete.

control to 1 .
77 MPa for 20% PKS & SCBA.Increase in the percentage of lime treated PKS & SCBA contents resulted in the reduction of the splitting tensile strength while there was an increase in the splitting tensile strength with curing age.This reduction can be caused by high water absorption characteristics of PKS and SCBA which lead to poor workability by creating voids in concrete.It is also due to lower specific gravity of PKS and SCBA which lead to lower concrete Open Journal of Civil Engineering density as compare to control.

Figure 17 .
Figure 17.Tensile splitting strength of lime treated PKS concrete.

Figure 19 .
Figure 19.Splitting tensile strength of PKS and SCBA concrete.

Table 1 .
Summary characteristics of PKS, coarse aggregate, and fine aggregate.

Table 2 .
Chemical properties of SCBA and OPC.
It could be noticed that the control mix has the highest compressive strength.The compressive strength decreased at respective Open Journal of Civil Engineering